Available online at www.sciencedirect.com
Solar Energy 86 (2012) 541–547 www.elsevier.com/locate/solener
Eﬀective conversion eﬃciency enhancement of solar cell using ZnO/PS antireﬂection coating layers Khaldun A. Salman ⇑, Khalid Omar, Z. Hassan Nano-Optoelectronics Research and Technology Laboratory, School of Physics, University Sains Malaysia, Penang 11800, Malaysia Received 13 July 2011; received in revised form 14 October 2011; accepted 29 October 2011 Available online 3 December 2011 Communicated by: Associate Editor Takhir Razykov
Abstract Zinc oxide (ZnO) ﬁlm was deposited on a porous silicon (PS) layer using a radio frequency sputtering system while the PS layer was prepared by a photoelectrochemical etching method. The ZnO/PS layers were found to be an excellent antireﬂection coating (ARC), exhibiting exceptional light trapping at wavelengths ranging from 400 to 1000 nm because of their lowest eﬀective reﬂectance. This, in turn, leads to increase the eﬃciency of solar cell to 18.15%. The ZnO ﬁlm was highly oriented with the c-axis perpendicular to the PS layer. The average crystallite size of the PS and ZnO/PS layers were 17.06 and 17.94 nm, respectively. Photoluminescence emission peaks proved the nanocrystalline characteristic of the PS layer and the ZnO ﬁlm. Raman measurements of the ZnO/PS layers were determined at room temperature and indicate that a high-quality ZnO nanocrystalline ﬁlm was formed. In the current paper, ZnO/PS ARC layers are attractive and oﬀer a promising technique to produce high-eﬃciency, low-cost solar cells. Ó 2011 Elsevier Ltd. All rights reserved. Keywords: Eﬃciency; Solar cell; Zinc oxide; Porous silicon; Anti-reﬂection coating
1. Introduction A porous silicon (PS) layer formed on a crystalline silicon (c-Si) wafer using electrochemical etching exhibits photoluminescent and electroluminescent properties similar to those of semiconductors with a direct energy band gap (Canham, 1990). The main improvement in the performance of the PS layers is the rough surface and low eﬀective refractive index compared with c-Si, which can decrease the reﬂective loss of solar radiation and lead to an increase of approximately 15–20% of the short-circuit current density (Jsc) of solar cells (Yae et al., 2006; Vitanov et al., 1997; Ueda et al., 1988). PS layers have become an attractive material for solar cells because of their band gap broadening, wide optical transmission ranging from 700 to 1000 nm, and surface roughness (Koshida and ⇑ Corresponding author. Tel.: +60 175373031; fax: +60 46579150.
E-mail address: [email protected]
(K.A. Salman). 0038-092X/$ - see front matter Ó 2011 Elsevier Ltd. All rights reserved. doi:10.1016/j.solener.2011.10.030
Koyama, 1992). PS layers are an excellent antireﬂection coating (ARC) for solar cells (Ben Ranha and Bessais, 2010). The ARC can enhance the eﬃciency of solar cells by increasing light trapping in the active region (Yoo, 2010; San Vicente et al., 2011). In the last couple of years, many researchers have increasingly focused on zinc oxide (ZnO) because of its multiple applications, such as laser diodes (Ye et al., 2007), transparent conductive contacts (Wong and Searson, 1999), and solar cells (Bahadur et al., 1986; Sil and Chakrabarti, 2010; Lu et al., 2010). ZnO has a direct band gap (3.37 eV), a high exciton binding energy (60 meV) at room temperature (RT), and a wurtzite crystal structure (Pawar et al., 2011). Recently, ZnO has attracted attention as one of the materials for the ARC of solar cells because it has good transparency and an appropriate refractive index (Yun-Ju et al., 2008; Kawakami et al., 2003; Kim and Kim, 2003; Liu et al., 2001; Greene et al., 2005; Tak and Yong, 2005; Chen and Gao, 2006; Riaz
K.A. Salman et al. / Solar Energy 86 (2012) 541–547
et al., 2009; Chen and Sun, 2010b). The integration of ZnO ﬁlms and c-Si samples is important. However, the deposition of high-quality ZnO ﬁlms on c-Si samples introduces stress between the materials because of the large mismatch in lattice constants and thermal expansion coeﬃcients (Hsu et al., 2005). Despite these problems, ZnO thin ﬁlms have been successfully deposited on spherical solar cells as an ARC with an eﬃciency of 11.8% (Minemoto et al., 2007). The PS layer is a convenient material for accommodating the deposition of ZnO ﬁlm onto pores in the layer because the PS layer has a large internal surface area, high resistance, and strong absorbability (Bisi et al., 2000). The integration of ZnO ﬁlms and a PS layer is more important because the deposition of high-quality ZnO ﬁlms on a PS layer can introduce a large matching of lattice constants and thermal expansion coeﬃcients (Chen and Sun, 2010b). Diﬀerent methods have been proposed to deposit ZnO ﬁlms on PS layers, such as chemical vapor deposition (Haga et al., 2001), a sol–gel process (Fujihara et al., 2001), direct current sputtering (Harding et al., 1991), and Radio Frequency (RF) sputtering (Cai et al., 2009; Choi et al., 2010; Vasanelli et al., 1987). In the present work, a ZnO ﬁlm was deposited on a PS layer using an RF sputtering system, and the PS layer was prepared by the photoelectrochemical etching (PECE) process. The objective of this work was to fabricate a high-eﬃciency solar cell using the ZnO/PS ARC layer technique. The authors suggest using ZnO/PS layers as a promising ARC to enhance and increase the light conversion eﬃciency of solar cells. 2. Experimental A PS layer was fabricated by PECE process of an n-type c-Si (1 0 0) wafer with a resistivity of 1–20 X cm and a thickness of 356–406 lm. Initially, the c-Si wafer was cleaned to remove the oxide layer using the Radio Corporation of America method. The PECE cell had a circular aperture at the bottom sealed with the c-Si sample. The cell, made of Teﬂon, was
a two-electrode system connected to the c-Si sample as the anode and platinum (Pt) as the cathode (Fig. 1). The c-Si sample was placed in an electrolyte solution HF (48%):C2H5OH (98%), 1:4 (by volume) to enable conduction of electrons inside the solution. A current density of 60 mA/cm2 and an etching time of 20 min were used to prepare the PS layer. Illumination was provided by a 150 W Xenon lamp positioned over the c-Si sample for maximum possible illumination. The synthesis was carried out at RT. Finally, the sample was rinsed in ethanol and air-dried after the etching process. To fabricate the solar cell, the sample was coated with photoresist. Next, a mask was placed directly above the PS layer and exposed to ultraviolet (UV) radiation for 40 s to form a patterned coating. P-type doping was achieved using the spin coating method by placing boron liquid on the center of the PS layer, followed by spin coating at RT at a speed of 1000 rpm for 10 s. The layer was then placed in a furnace at 100 °C for 15 min to remove moisture. Dopant diﬀusion was accomplished using a tube furnace at 1000 °C for 60 min under ﬂowing (4 L/min) nitrogen gas. The 135 nm-thick ZnO ﬁlm was deposited on the PS layer by RF sputtering with a power of 200 W at ambient temperature using an A500 EDWARDS sputtering unit. The growth conditions of the ZnO ﬁlm deposited onto the PS layer are summarized in Table 1. Annealing of the ZnO/PS layers was done at 500 °C for 30 min under ﬂowing (4 L/min) nitrogen gas. Annealing improved the quality and optical properties of the ZnO ﬁlm. Silver evaporation was used on the p-type of the sample to form a metallization grid pattern, and aluminum evaporation was used on the n-type to form a reﬂector contact. Annealing was carried out at 400 °C for 20 min to insure optimal contact. Scanning electron microscopy (SEM) and energy dispersive X-ray (EDX) analysis (JSM-6460 LV, Japan) were used to determine the surface morphology and composition of the PS and ZnO/PS layers, respectively. X-ray diﬀraction (XRD) measurements were carried out using a highresolution X-ray diﬀractometer system (PANalytical X’pert
Table 1 RF sputtering conditions for ZnO ﬁlm deposition.
Fig. 1. The photoelectrochemical etching (PECE) cell set up.
Target diameter Distance between the target and substrate Substrate Substrate temperature Ultimate pressure Vacuum (plasma) pressure Gas RF sputtering power Deposition rate Deposition time The required thickness of ZnO ﬁlm
7.5 cm 10 cm PS layer 25 °C 1 106 mbar 1.74 102 mbar Ar 99.99% 200 W Dr2 0.20 A°s 13 min 135 nm
K.A. Salman et al. / Solar Energy 86 (2012) 541–547
PRO MRD PW3040, Almelo, The Netherlands) to determine the ZnO crystallite structure using Cu Ka radiation with a wavelength of 0.15406 nm. Photoluminescence (PL) and Raman studies were carried out using a spectroscopy system (Jobin Yvon HR 800 UV, Edison, NJ, USA). Optical reﬂectance of the c-Si sample, PS, and ZnO/PS layers were obtained using an optical reﬂectometer (Filmetrics, F20, USA). I–V characteristics were studied under the air mass 1.5 global (AM 1.5G) illumination condition (Chen and Sun, 2010a). 3. Results and discussions Fig. 2 shows the pores randomly distributed on the PS surface. Some pores appeared star-like and had elongated shapes with an average diameter of 6.2 nm, as calculated using the following equation (Ossicini et al., 2003). h2 1 1 EðeVÞ ¼ Eg þ 2 þ ; ð1Þ 8d me mh where E(eV) = 1.81 eV is the energy band gap of PS obtained from the PL peak of the PS layer as shown in the inset of Fig. 6, Eg = 1.12 eV is the energy band gap of c-Si, h is Planck’s constant = 4.13 1015 eV s, d is the diameter of the pore, and me and mh are the electron and hole eﬀective mass, respectively (at 300 K, me ¼ 0:19mo ; mh ¼ 0:16mo , and mo = 9.109 1031 kg). Moreover, the surface of the PS layer was etched completely. The formation of numerous, new, tiny pores inside the initial pores and above the pore walls can be clearly distinguished, which increased the porosity (P) of the PS layer to 91% according to the following equation (Hyunwoo et al., 2006): m1 m2 P ð%Þ ¼ ; ð2Þ m1 m3 where m1 and m2 are the sample weight before and after anodization, respectively; and m3 is the sample weight after removing the PS layer using a 3% KOH solution in 50 s (Fay¨ and Shah, 2008). The ZnO ﬁlm was deposited on the PS layer by RF sputtering as shown in the SEM image in Fig. 3. The deposition
Fig. 2. SEM image of the PS layer.
Fig. 3. SEM image of ZnO/PS layers.
of ZnO inside the pores along the walls partially ﬁlled or covered the pores. Fig. 4 shows the EDX spectrum and atomic composition of the ZnO/PS layers. A description of the atomic composition of the elements in the layers is given by the percentage, as shown in the inset table in Fig. 4. The concentrations of these elements are indicated by the peaks, and it is very clear that the elements corresponding to the peaks comprised the layer. Carbon was detected as a contaminant in the sample. Fig. 5 shows that the ZnO/PS layers exhibited a dominant diﬀraction peak at 2h = 69.0978° corresponding to the PS (1 0 0) layer (Minemoto et al., 2007). The diﬀraction peak at 34.2398° corresponds to the (0 0 2) plane of the ZnO ﬁlm, indicating that the ZnO nanocrystalline ﬁlm was highly oriented along the c-axis vertical to the PS layer (Chen and Sun, 2010b). The diﬀraction peak at 44.3560° is related to Si Carbide (SiC) from the XRD sample holder (Hassan et al., 2011). The sharp diﬀraction peak from the ZnO ﬁlm with a weak FWHM of 0.29 [2h] indicates the high quality of the ZnO ﬁlm. The average crystallite size was calculated using the Debye–Scherrer formula as follows (Cullity, 1959): D¼
0:9k ; B cos h
where D is the average grain size, k is the X-ray radiation wavelength (0.15406 nm), h is the diﬀraction Bragg angle and B is the FWHM value in the radians unit. The FWHM value obtained from XRD peak for PS layer was 9.8696 1003 radians and for the ZnO ﬁlm was 8.0930 1003 radians. The values of average crystallite size obtained from XRD were 17.06 nm for the PS layer and 17.94 nm for the ZnO ﬁlm. The decrease in average crystallite size indicated an increase in the porosity of the PS layer (Yon et al., 1987). In addition, the strain (ezz) of the nanocrystalline ZnO ﬁlm grown on the PS layer along the c-axis can be calculated using the following equation (Tsay et al., 2010): c co ezz ð%Þ ¼ ; ð4Þ co
K.A. Salman et al. / Solar Energy 86 (2012) 541–547
Fig. 4. EDX spectra of ZnO/PS layers.
Fig. 5. XRD spectrum of the ZnO/PS layers.
Fig. 6. PL spectra of ZnO/PS layers.
where c is the lattice constant of the strained ZnO ﬁlm calculated from XRD data, and co is the unstrained lattice constant for ZnO. The obtained value of strain is 0.36%. A positive value is associated with tensile strain (Ghosh and Basak, 2004). The low value of the tensile strain
revealed that the ZnO nanocrystalline ﬁlm preferred to grow along the c-axis, and gave evidence of a high-quality crystal resulting from a small lattice mismatch between the ZnO ﬁlm and the PS (1 0 0) layer (9.9%) compared with (39–40.2)% between the ZnO ﬁlm and c-Si (1 0 0) obtained by the sputtering method (Phan and Chung, 2011; Gopalakrishnan et al., 2006). The PL spectra of the PS and the ZnO/PS layers were measured by a He–Cd excitation laser source at 325 nm at RT (Fig. 6). The PL spectrum of the PS layer (shown as an inset in Fig. 6) shows a very intense PL emission peak at 683.5 nm, which revealed the good quality of the PS layer (Chen and Chen, 1999). The left PL peak at 387.5 nm UV emission was caused by the near band edge emission in the wide band gap of the ZnO which resulted from the direct recombination of photogenerated charge carriers (Yu et al., 2009; Umar et al., 2006). The original value of the PL peak of the bulk ZnO was 367.655 nm (Steiner, 2004). Therefore, the red shift in the PL peak of ZnO ﬁlm toward a longer wavelength of 387.5 nm was attributed to Zn vacancies in the ZnO energy band gap. Moreover, we believe that contamination of the ZnO/PS layers caused the red shift in the PL peak of the ZnO ﬁlm (Fig. 6) (Hyunwoo et al., 2006). The right, high-intensity PL peak at 637.5 nm (red emission) is attributed to the PS layer (Liu et al., 2003). The blue shift in the PL peak of the PS layer toward a shorter wavelength of 637.5 nm is attributed to the quantum conﬁnement eﬀect of electrons in nanosized particles in the PS layer (Chen and Chen, 1999; Hummel et al., 1995). In addition, the observed emission at 637.5 nm is related to the surface oxidation by ZnO deposition (Kayahan, 2010). The red emission peak for the PS layer containing a shoulder peak of 605 nm (yellow orange emission) in the visible (VIS) region is related to the high number of intrinsic structural defects resulting from Zn vacancies (Jayakumar et al., 2010).
K.A. Salman et al. / Solar Energy 86 (2012) 541–547
As a result of the high porosity of the PS layer, the blue shift in the PL peak is possible and the high intensity of the strong red emission will occur from the PS layer (Umar et al., 2006; Liu et al., 2003; Prabakaran et al., 2008). In other words, in low-dimensional structures, the probability of the recombination of electrons and holes will be higher, leading to an increase in optical conﬁnement energy and, ﬁnally, an increase in photo-conversion eﬃciency (Wu et al., 2000). Raman spectra of all layers were measured by an Argon–Ion excitation laser source at 514.5 nm at RT (Fig. 7). A sharp solid line was formed in the c-Si sample spectrum with an FWHM of 3.0 cm1 at 521 cm1 because of the scattering of ﬁrst-order phonons (Liu et al., 2003). The penetration depth of the Argon–Ion laser is greater than the thickness of the ZnO ﬁlm; hence, the spectrum of the PS layer displayed a very strong Raman intensity peak that red-shifted and became broader at 517 cm1 with an FWHM of 8.6 cm1 compared with the c-Si sample. The observed phonon frequency at 302 cm1 was also related to the c-Si substrate in the ZnO/PS layers (Hassan et al., 2011), which has a broadened FWHM and a high intensity compared with the c-Si sample and the PS layer as shown in the inset of Fig. 7. The formation of the PS layer led to a peak-shift asymmetry and an increase in the peak intensity. This feature of Si nanocrystals is attributed to the quantum conﬁnement of optical phonons in the electronic wave function of Si nanocrystals (Vinod and Lal, 2005). The ZnO wurtzite hexagonal crystal structure belongs to space group C 46m in the group theory with two formula units per primitive cell (Vinod and Lal, 2005). Therefore, the Raman-active zone center for optical phonons is 2A1 + 2B1 + 2E1 + 2E2, where A1 and E1 symmetry are polar phonon modes with two diﬀerent frequencies for transverse-optical (TO) and longitudinal-optical (LO) phonons, respectively. The 2B1 are silent modes.
The E2 symmetry is a nonpolar phonon mode with two frequencies: E2 (high), related to oxygen atoms, and E2 (low), related to the zinc sub-lattice (Alim et al., 2005). The E2 (high) mode appears as two bands at 442 and 492 cm1 related to E2 (high) due to oxygen atoms present after the ZnO deposition (Vinodkumar et al., 2010). Fig. 8 shows the reﬂection spectra of all layers compared with the c-Si sample. The PS layer consists of nano-silicon crystals and nano-pores. Therefore, the refractive index was decreased and controlled by the pores with respect to the high porosity, leading to a decrease in reﬂection (Aspnes et al., 1979). The PS reduced light reﬂection at wavelengths ranging from 400 to 1000 nm compared with the reﬂectivity of the c-Si sample. The lowest eﬀective reﬂectance was obtained from the ZnO/PS layers, which clearly reduced light reﬂection and increased light trapping at wavelengths ranging from 400 to 1000 nm compared with the reﬂectivity of the c-Si sample and PS layer. The synthesis of ZnO/PS ARC layers in the solar cells enhanced the photo-conversion process with high transparency and increased light absorption in the near-UV/VIS region of the solar spectrum. This is expected to increase the eﬃciency of solar cells compared with the solar cell without and with a PS ARC layer, respectively (Fig. 9) because the transparency and trapping of the incident radiation resulted from the passivation and heterogeneous properties of the ZnO/PS ARC layers. The solar cells were characterized under a 100 mW/cm2 illumination condition. The I–V measurements of the solar cells with ZnO/PS ARC layer conﬁrmed that Isc increased from 14.46 and 33.90 to 35.50 mA/cm2 and Voc increased from 367.20 and 595.00 to 627.30 mV compared with the solar cell without and with a PS ARC layer, respectively. This leads to an 18.15% increase in conversion eﬃciency compared with 3.64% and 15.50% for the solar cell without and with a PS ARC layer, respectively.
Fig. 7. Raman spectra of ZnO/PS layers compared to the c-Si sample.
Fig. 8. Reﬂection spectra of the ZnO/PS layers compared to the c-Si sample and the PS layer.
K.A. Salman et al. / Solar Energy 86 (2012) 541–547
eﬃciency of the commercial solar cells with standard alkaline-textured pyramids and SiNx single-ARC layer. Acknowledgment The authors would like to thank the research university (RU) grant, Universiti Sains Malaysia, and JUST-Jordan and TWAS-Italy Associteship for their support. References
Fig. 9. Current–Voltage curves of solar cells with ZnO/PS ARC layers compared with and without a PS ARC layer.
Table 2 Current–Voltage measurements of solar cells with ZnO/PS ARC layers compared with and without a PS ARC layer. Solar cells
With ZnO/PS ARC layers With PS ARC layer Without PS ARC layer
503.00 30.82 287.90 12.67
595.00 33.90 367.20 14.46
76.40 15.50 68.65 3.64
Im Voc (mA/cm2) (mV)
Isc FF (mA/cm2) (%)
In the present work, the solar cell with ZnO/PS ARC layers displayed increases in (Isc), (Voc), and conversion eﬃciency compared with the solar cell with and without a PS ARC layer (Table 2). 4. Conclusions The surface morphology of the PS and ZnO/PS layers was characterized using SEM. Nano-pores with an average diameter of 6.2 nm were produced in the PS layer using the PECE process. This resulted in an increase in porosity up to 91%. The ZnO ﬁlm was successfully deposited inside the nano-pores of the PS layer along the walls in order for the pores to be partially ﬁlled or covered using the RF sputtering system. The ZnO ﬁlm was highly oriented with the c-axis perpendicular to the PS layer. The average crystallite size of the PS and ZnO ﬁlm was 17.06 and 17.94 nm, respectively. The PL emission peaks proved the nanocrystalline characteristic of the PS layer and the ZnO ﬁlm. In addition, a high-quality ZnO nanocrystalline ﬁlm was formed. The lowest eﬀective reﬂectance was obtained for the ZnO/PS layers. These layers were found to be an excellent ARC in enhancing and increasing the light conversion eﬃciency of solar cells to 18.15%, which is close to the
Alim, K.A., Fonoberov, V.A., Shamsa, M., Balandina, A.A., 2005. MicroRaman investigation of optical phonons in ZnO nanocrystals. J. Appl. Phys. 97, 124313–124317. Aspnes, D.E., Theeten, J.B., Hottier, F., 1979. Investigation of eﬀectivemedium models of microscopic surface roughness by spectroscopic ellipsometry. Phys. Rev. B 20, 3292–3302. Bahadur, L., Hamdani, M., Koenig, J.F., Chartier, P., 1986. Studies on semiconducting thin ﬁlms prepared by the spray pyrolysis technique for photoelectrochemical solar cell applications: Preparation and properties of ZnO. Sol. Energ. Mater. 14, 107–120. Ben Ranha, M., Bessais, B., 2010. Enhancement of photovoltaic properties of multicrystalline silicon solar cells by combination of buried metallic contacts and thin porous silicon. Sol. Energy 84, 486–491. Bisi, O., Ossicini, S., Pavesi, L., 2000. Porous silicon: a quantum sponge structure for silicon based optoelectronics. Surf. Sci. Rep. 38, 1–126. Cai, H., Shen, H., Yin, Y., Lu, L., Shen, J., Tang, Z., 2009. The eﬀects of porous silicon on the crystalline properties of ZnO thin ﬁlms. J. Phys. Chem. Solids 70, 967–971. Canham, T.L., 1990. Silicon quantum wire array fabrication by electrochemical and chemical dissolution of wafers. Appl. Phys. Lett. 57, 1046– 1048. Chen, C.H., Chen, Y.F., 1999. Strong and stable visible luminescence from Au-passivated porous silicon. Appl. Phys. Lett. 75, 2560–2562. Chen, Z., Gao, L., 2006. A facile route to ZnO nanorod arrays using wet chemical method. J. Cryst. Growth 293, 522–527. Chen, J.Y., Sun, K.W., 2010a. Enhancement of the light conversion eﬃciency of silicon solar cells by using nanoimprint anti-reﬂection layer. Sol. Energy Mater. Sol. Cells 94, 629–633. Chen, J.Y., Sun, K.W., 2010b. Growth of vertically aligned ZnO nanorod arrays as antireﬂection layer on silicon solar cells. Sol. Energy Mater. Sol. Cells 94, 930–934. Choi, J.-H., Das, S.N., Moon, K.-J., Kar, J.P., Myoung, J.-M., 2010. Fabrication and characterization of p-Si nanowires/ZnO ﬁlm heterojunction diode. Solid-State Electron. 54, 1582–1585. Cullity, B.D., 1959. Elements of X-ray Diﬀraction. Addison-Wesley, London. ¨ , S., Shah, A., 2008. Zinc oxide grown by CVD process as transparent FaY contact for thin ﬁlm solar cell applications. In: Ellmer, K., Klein, A., Rech, B. (Eds.), Transparent Conductive Zinc Oxide. Springer, Berlin Heidelberg, pp. 235–302. Fujihara, S., Sasaki, C., Kimura, T., 2001. Crystallization behavior and origin of c-axis orientation in sol-gel-derived ZnO:Li thin ﬁlms on glass substrates. Appl. Surf. Sci. 180, 341–350. Ghosh, R., Basak, D., 2004. Eﬀect of substrate-induced strain on the stractural, electrical, and optical properties of polycrystalline ZnO thin ﬁlms. J. Appl. Phys. 96, 2689–2692. Gopalakrishnan, N., Shin, B.C., Lim, H.S., Kim, G.Y., Yu, Y.S., 2006. Comparison of ZnO:GaN ﬁlms on Si(1 1 1) and Si(1 0 0) substrates by pulsed laser deposition. Phys. B, 756–759 (Amsterdam, Neth.). Greene, L.E., Law, M., Tan, D.H., Montano, M., Goldberger, J., Somorjai, G., Yang, P., 2005. General route to vertical ZnO nanowire arrays using textured ZnO seeds. Nano Lett. 5, 1231–1236. Haga, K., Wijesena, P.S., Watanabe, H., 2001. Group III impurity doped ZnO ﬁlms prepared by atmospheric pressure chemical-vapor deposi-
K.A. Salman et al. / Solar Energy 86 (2012) 541–547 tion using zinc acetylacetonate and oxygen. Appl. Surf. Sci. 169–170, 504–507. Harding, G.L., Window, B., Horrigan, E.C., 1991. Aluminium-and indium-doped zinc oxide thin ﬁlms prepared by DC magnetron reactive sputtering. Sol. Energ. Mater. 22, 69–91. Hassan, J.J., Hassan, Z., Abu-Hassan, H., 2011. High-quality vertically aligned ZnO nanorods synthesized by microwave-assisted CBD with ZnO-PVA complex seed layer on Si substrates. J. Alloys Compd. 509, 6711–6719. Hsu, H.-C., Cheng, C.-S., Chang, C.-C., Yang, S., Chang, C.-S., Hsieh, W.-F., 2005. Orientation-enhanced growth and optical properties of ZnO nanowires grown on porous silicon substrates. Nanotechnology 16, 297–301. Hummel, R.E., Ludwig, M.H., Chang, S.S., 1995. Strong, blue, roomtemperature photoluminescence of spark-processed silicon. Solid State Commun. 93, 237–241. Hyunwoo, L., Lee, E., Soohong, L., 2006. Investigation of nano-porous silicon antireﬂection coatings for crystalline silicon solar cells. Nanotechnology Materials and Devices Conference. NMDC 2006. IEEE, Gyeongju, Korea. pp. 340–341. Jayakumar, O.D., Sudarsan, V., Sudakar, C., Naik, R., Vatsa, R.K., Tyagi, A.K., 2010. Green emission from ZnO nanorods: Role of defects and morphology. Scr. Mater. 62, 662–665. Kawakami, M., Hartanto, A.B., Okada, Y.N.T., 2003. Synthesis of ZnO nanorods by nanoparticle assisted pulsed-laser deposition. J. Appl. Phys. 42, 33–35. Kayahan, Ersin, 2010. White light luminescence from annealed thin ZnO deposited porous silicon. J. Lumin. 130, 1295–1299. Kim, K.-S., Kim, H.W., 2003. Synthesis of ZnO nanorod on bare Si substrate using metal organic chemical vapor deposition. Phys. B 328, 368–371. Koshida, N., Koyama, H., 1992. Visible electro- and photoluminescence from porous silicon and its related optoelectronic properties. Mater. Res. Soc. Symp. Proc. 256, 219–222. Liu, R., Vertegel, A.A., Bohannan, E.W., Sorenson, T.A., Switzer, J.A., 2001. Epitaxial electrodeposition of zinc oxide nanopillars on single crystal gold. Chem. Mater. 13, 508–512. Liu, Y.L., Liu, Y.C., Yang, H., Wang, W.B., Ma, J.G., Zhang, J.Y., Lu, Y.M., Shen, D.Z., Fan, X.W., 2003. The optical properties of ZnO ﬁlms grown on porous Si templates. J. Phys. D: Appl. Phys. 36, 2705– 2708. Lu, L., Li, R., Fan, K., Peng, T., 2010. Eﬀects of annealing conditions on the photoelectrochemical properties of dye-sensitized solar cells made with ZnO nanoparticles. Sol. Energy 84, 844–853. Minemoto, T., Mizuta, T., Takakura, H., Hamakawa, Y., 2007. Antireﬂective coating fabricated by chemical deposition of ZnO for spherical Si solar cells. Sol. Energy Mater. Sol. Cells 91, 191– 194. Ossicini, S.L., Pavesi, L., Priolo, F., 2003. Light emitting silicon for microphotonics. Springer-Verlag, Berlin Heidelberg. Pawar, R.C., Shaikh, J.S., Babar, A.A., Dhere, P.M., Patil, P.S., 2011. Aqueous chemical growth of ZnO disks, rods, spindles and ﬂowers: pH dependency and photoelectrochemical properties. Sol. Energy 85, 1119–1127. Phan, D.-T., Chung, G.-S., 2011. Comparison of ZnO thin ﬁlms grown on a polycrystalline 3C-SiC buﬀer layer by RF magnetron sputtering and a sol–gel method. Appl. Surf. Sci. 257, 3285–3290. Prabakaran, R., Peres, M., Monteiro, T., Fortunato, E., Martins, R., Ferreira, I., 2008. The eﬀects of ZnO coating on the photoluminescence properties of porous silicon for the advanced optoelectronic devices. J. Non-Cryst. Solids 354, 2181–2185.
Riaz, M., Fulati, A., Amin, G., Alvi, N.H., Nur, O., Willander, M., 2009. Buckling and elastic stability of vertical ZnO nanotubes and nanorods. J. Appl. Phys. 109, 034309–034314. San Vicente, G., Bayo´n, R., Germa´n, N., Morales, A., 2011. Surface modiﬁcation of porous antireﬂective coatings for solar glass covers. Sol. Energy 85, 676–680. Sil, D., Chakrabarti, S., 2010. Photocatalytic degradation of PVC-ZnO composite ﬁlm under tropical sunlight and artiﬁcial UV radiation: A comparative study. Sol. Energy 84, 476–485. Steiner, T., 2004. Semiconductor nanostructures for optoelectronic applications. Artech House Inc, Norwood. Tak, Y., Yong, K., 2005. Controlled growth of well-aligned ZnO nanorod array using a novel solution method. J. Phys. Chem. B 109, 19263– 19269. Tsay, C.-Y., Fan, K.-S., Chen, S.-H., Tsai, C.-H., 2010. Preparation and characterization of ZnO transparent semiconductor thin ﬁlms by sol– gel method. J. Alloys Compd. 495, 126–130. Ueda, K., Nakato, Y., Tsubomura, H., 1988. Eﬃcient and stable solar to chemical conversion with n+-p junction crystalline silicon electrodes having textured surfaces. Sol. Energ. Mater. 17, 37–46. Umar, A., Karunagaran, B., Suh, E.-K., Hahn, Y.B., 2006. Structural and optical properties of single-crystalline ZnO nanorods grown on silicon by thermal evaporation. Nanotechnology 17, 4072–4077. Vasanelli, L., Valentini, A., Losacco, A., 1987. Preparation of transparent conducting zinc oxide ﬁlms by reactive sputtering. Sol. Energ. Mater. 16, 91–102. Vinod, P.N., Lal, M., 2005. Surface and optical characterization of the porous silicon textured surface for application in photovoltaics. Photovoltaic Specialists Conference, 2005. Conference Record of the Thirty-ﬁrst IEEE, 3–7 January 2005, pp. 1135–1138. Vinodkumar, R., Navas, I., Chalana, S.R., Gopchandran, K.G., Ganesan, V., Philip, R., Sudheer, S.K., Mahadevan Pillai, V.P., 2010. Highly conductive and transparent laser ablated nanostructured Al: ZnO thin ﬁlms. Appl. Surf. Sci. 257, 708–716. Vitanov, P., Kamenova, M., Tyutyundzhiev, N., Delibasheva, M., Goranova, E., Peneva, M., 1997. High-eﬃciency solar cell using a thin porous silicon layer. Thin Solid Films 297, 299–303. Wong, E.M., Searson, P.C., 1999. ZnO quantum particle thin ﬁlms fabricated by electrophoretic deposition. Appl. Phys. Lett. 74, 2939– 2941. Wu, X.L., Xiong, S.J., Fan, D.L., Gu, Y., Bao, X.M., 2000. Stabilized electronic state and its luminescence at the surface of oxygenpassivated porous silicon. Phys. Rev. B 62, 7759–7762. Yae, S., Kobayashi, T., Kawagishi, T., Fukumuro, N., Matsuda, H., 2006. Antireﬂective porous layer formation on multicrystalline silicon by metal particle enhanced HF etching. Sol. Energy 80, 701–706. Ye, Z.Z., Lu, J.G., Zhang, Y.Z., Zeng, Y.J., Chen, L.L., Zhuge, F., Yuan, G.D., He, H.P., Zhu, L.P., Huang, J.Y., Zhao, B.H., 2007. ZnO lightemitting diodes fabricated on Si substrates with homobuﬀer layers. Appl. Phys. Lett. 91, 113503–113505. Yon, J.J., Barla, K., Herino, R., Bomchil, G., 1987. The kinetics and mechanism of oxide layer formation from porous silicon formed on pSi substrates. J. Appl. Phys. 62, 1042–1048. Yoo, J., 2010. Reactive ion etching (RIE) technique for application in crystalline silicon solar cells. Sol. Energy 84, 730–734. Yu, C.-F., Sung, C.-W., Chen, S.-H., Sun, S.-J., 2009. Relationship between the photoluminescence and conductivity of undoped ZnO thin ﬁlms grown with various oxygen pressures. Appl. Surf. Sci. 256, 792–796. Yun-Ju, L., Ruby, D.S., Peters, D.W., Mckenzie, B.B., Hsu, J.W.P., 2008. ZnO Nanostructures as eﬃcient antireﬂection layers in solar cells. Nano Lett. 8, 1501–1505.